study of inN surface by high resolution electron energy loss
Study of InN surface by high resolution electron energy loss spectroscopy (HREELS)
Ananta R. Acharya and Brian D. Thoms
Georgia State University, Department of Physics and Astronomy, Atlanta, GA 30303
Understanding the surface structure and termination of semiconductor thin films during epitaxial growth is critical since it affects the
structural, interfacial and electronic properties of epilayers and device structures. The structural properties and surface bonding configuration
of InN layers grown by high pressure chemical vapor deposition (HPCVD) have been characterized using high resolution electron energy loss
spectroscopy (HREELS). The HREELS analysis of these InN layers shows that the surface is predominantly terminated with NH2 species. This
is in contrast to previous work on HPCVD-grown InN layers, which showed only NH species on the nitrogen terminated surface. The presence
of NH2 related modes of vibration is the indication of the orientation of the surface other than c-plane.
Key words: HREELS, Indium nitride, NH2
of highly volatile compounds, such as InN, is possible if surface
InN, one of the group III nitride semiconductors, has been an
stabilization is done at high pressures. High pressure chemical vapor
interesting area of research due to its inherent properties which
deposition (HPCVD) has been found as an effective technique to
can increase the performance of photovoltaics, electronics and
grow stoichimetric InN layers at elevated temperatures(~900 0C).7
optoelectronics devices. It is a direct and narrow band gap (0.65
eV) semiconductor. Among all III-nitride semiconductors, InN
HREELS is a surface sensitive vibrational spectroscopic technique
has the lowest effective mass for electrons1 which leads to high
in which low energy electrons are incident on the surface of
mobility and high saturation velocity. Using InN and its alloys with
the sample. The scattered electrons are collected in a specular
GaN and AlN, emission of nitride-based LEDs can be extended
direction and energy is analysed. Electrons with energy loss up
from ultraviolet to near infrared region. For example, InGaN,
to 500 meV are counted to accumulate a spectrum. Our HREELS
a ternary alloy of InN and GaN, has been found very useful in
spectrometer consists of a cathode made of lanthanum hexaboride
optoelectronic devices, such as, LEDs2 and lasers.3 By changing
and a pair of cylindrical monochromators and analyzers. A
the In content, the band gap of InGaN can be tuned over a wide
symmetrical system of input-output zoom lenses are positioned
range corresponding to wavelengths from infrared to ultraviolet
between the monochromators and analyzers in order to focus,
region. This important property of InGaN alloy has made possible
accelerate or decelerate beam of electrons to and from the sample
to fabricate high efficiency photovoltaic cells capturing most of
surface. HREELS experiments were performed in a stainless-steel
the solar spectrum.4
ultrahigh vacuum (UHV) system with base pressure of 2x1010
Torr. The UHV system is also equipped with Auger electron
Despite the enticing properties for device fabrication, the growth
spectroscopy (AES), low energy electron diffraction (LEED) and
of high crystalline quality InN remains a challenge, especially due
ion gun apparatus. The chamber is pumped by three pumps; two
to two reasons: stoichiometric instability and low dissociation
turbo molecular pumps and one ion pump. The need of this much
temperature. Using low pressure chemical vapor deposition
low pressure is mainly to keep the surface clean and avoid any
(LPCVD) at low temperatures about 600 0C, thermal desorption is
kind of collisions or interactions with air molecules. The details of
suppressed.5 However, the cracking efficiency of ammonia in this
the UHV system and sample mount have already been reported by
temperature regime is extremely low and it requires a large group
Bellitto et al. 8
V-III precursor ratio.6 Even at high temperature regime, the growth
The Himalayan Physics
II. Study of InN surface by high resolution electron energy loss spectroscopy
The InN layers, characterized here, were grown by HPCVD process
in Dr. Dietz’s lab at Georgia State University in the department
of Physics and Astronomy. The sample was grown on a sapphire
substrate at a temperature of 865 0C, a reactor pressure of 15 bar,
and an ammonia (NH3) to trimethylindium (TMI) precursor ratio
of 3000. The sample was cleaned with acetone and rinsed with
isopropyl alcohol before installing into the UHV chamber. The
ultrahigh vacuum condition was restored in the chamber by a 5
day long baking and cooling method. After maintaining the UHV
environment in the chamber, the sample was cleaned by a procedure
of bombardment with 1 keV nitrogen ions followed by atomic
hydrogen cleaning (AHC), which was reported as an effective
technique to remove surface contaminants by Piper et al.9 AHC
Fig. 1. HREELS of InN after AHC. Spectra were acquired in the
was performed by backfilling the vacuum chamber with hydrogen
specular direction with an incident electron energy of 12.5 eV.
to a pressure of 8.4x10-7 Torr in the presence of a tungsten filament
heated to 1575 °C to produce H-atoms. The sample was kept at 20
In another work,11 HREELS spectra of the AHC treated InN layers
mm from the dosing filament for 5 minutes (giving an exposure
were observed as shown in Fig. 2. In this work, they varied the
of 250 L of hydrogen, 1 L= 1x10-6 Torr s). After 5 minutes, the
energy of the incident electrons and observed a strong loss feature
sample was heated to 350 °C by the bombardment of the electrons
at 560 cm-1 in all spectra. This loss feature was assigned to a
from the back of the sample mount for 10 minutes keeping the
Fuchs-Kliewer surface phonon. Most importantly, they observed
exposure of H-atom same as before (giving an additional exposure
a broad loss feature in the range of 3100-3600 cm-1 for different
of 500 L of hydrogen). In order to monitor the surface cleanliness,
incident electron energies which they assigned to a conduction
Auger electron spectroscopy (AES) was used. The procedure of
band plasmon excitation. From these spectra they revealed the fact
cleaning was repeated until the surface of the sample was free
of the presence of a surface electron accumulation.
from contaminants as confirmed by AES. After the sample was
found in good shape, HREELS experiments were performed in a
specular geometry with an incident and scattered angle of 600 from
the surface normal, and an incident electron beam energy of 5.6
III. RESULTS AND DISCUSSION
Fig. 1 shows the HREELS spectra of InN epilayers grown on
GaN/sapphire studied by authors’ research group previously.10 The
strong loss feature at 550 cm-1 was assigned to a Fuchs- Kliewer
surface phonon. The loss peak at 3260 cm-1 for the atomic hydrogen
cleaned (AHC) surface was assigned to an N-H stretching vibration,
while the loss feature at 870 cm-1 was assigned to an N-H bending
vibration. In addition, the peak near 360 cm-1 was suggested to the
bouncing vibrations of the nitrogen surface atoms with the surface.
Fig. 2. HREELS from an atomic hydrogen cleaned InN sample
From these observations it was concluded that the InN film in that
with incident electron energies of (a) 7 eV, (b) 15 eV, (c) 25 eV,
work was N-polar and N-H terminated.
and (d) 35 eV.
The Himalayan Physics
Ananta R. Acharya and Brian D. Thoms
In the present work, the HREELS spectrum of an InN sample
obtained after AHC is depicted in Fig. 3. As shown in Fig. 3, loss
features are observed at 640 cm-1, 1260 cm-1, 1440 cm-1, 1600 cm-1,
2960 cm-1, 3400 cm-1 and 3710 cm-1. The loss peaks at 1260, 1600
and 3400 cm-1 indicate that this surface is predominantly NH2
terminated as opposed to the N-H termination observed in earlier
work.10-11 Unlike in the previous work10 where they observed
Fuchs-Kliewer surface phonon at 550 cm-1, a strong and broad loss
feature is observed at 640 cm-1 in the present work. Tindall et al.12
reported a rocking mode of NH2 vibration at 884cm-1 on Ge(100)
surface. The strong and broad loss feature at 640 cm-1 is assigned
to the unresolved overlap of the Fuchs-Kliewer surface phonon
and the rocking mode of the NH2 vibration. The loss feature at
3400 cm-1 is assigned to an NH2 stretching vibration in agreement
with that assigned by Tanaka et al.13 for NH2 symmetric stretching
vibration on InP(110). The loss features at 1260 cm-1 and at 1600
cm-1 are assigned to NH2 wagging and scissor modes of vibration
respectively which have close agreement with those assigned by
Tindall et al.12 on Ge(100).
HREEL spectra of HPCVD-grown InN after atomic
Small loss features at 1440 cm-1 and at 2960 cm-1 have been
assigned to the bending and stretching modes of C-H vibrations
respectively. A small loss feature at 3710 cm-1 is assigned to stretch
mode of O-H vibration. The loss feature at 3400 cm-1 is assigned
to an NH2 stretching vibration in agreement with that assigned by
Tanaka et al.13 for NH2 symmetric stretching vibration on InP(110).
Nienhaus et al.14 reported InH stretching vibration at 1650-1700
cm-1 in HREELS experiments and at 1630-1650 cm-1 from ab initio
calculations15 on InP surfaces. However, no loss feature in this
range was observed in the present work indicating no surface InH,
i.e. no metallic indium on the surface. In the HREEL spectrum, the
appearance of the loss features related to NH2 species implies that
the surface is predominantly N-terminated. Since no evidence of
metallic indium is observed in our HREELS spectrum, it can be
concluded that the presence of NH2 species on InN layer is due to
the tilted facets.
In summary, InN surface grown by HPCVD has been characterized
using HREELS. The termination of the surface depends upon the
growth parameters and the type of the substrate. The HREEL
spectrum shows that the InN surface is mainly NH2 terminated.
The presence of NH2 bonds at the InN surface is directly related to
tilted InN facets and is not observed on the c-plane InN surface.
S.N. Mohammad and H. Morkoc, 1996. Prog. Quantum
Electron 20, 361.
I. Akasaki, H. Amano, N. Koide, M. Kotaki, and K.
Manabe, 1993. Physica B 185, 428.
S. Nakamura, M. Senoh, S. Nagahama, N. Iwasa,
T. Yamada, T. Matsushita, H. Kiyoku, and Y.
Sugimoto,1994. Jpn. J. Appl. Phys. 75, 7365.
Akio Yammoto, Md. R. Islam, Ting-Ting Kang, and
Akihiro Hashimoto, 2010. Phys. Stat. Sol. (c), 1-8
A.G Bhuiyan, A. Hashimoto, and A. Yamamoto, 2003. J.
Appl. Phys. 94 , p.2779-2808.
N. Dietz, M. Strassburg, and V. Woods,2005. J. Vac. Sci.
Technol. A 23, 1221.
N. Dietz, in III-Nitrides Semiconductor Materials,
edited by Z. C. Feng Imperial College Press, pp. 203–
V. J. Bellitto, B. D. Thoms, D. D. Koleske, A. E.
Wickenden, R. L. Henry, Surf. Sci. 430, 80 (1999).
L. F. J. Piper, T. D. Veal, M. Walker, I. Mahboob, C.
F. McConville, H. Lu, and W. J. Schaff, J. Vac. Sci.
Technol. A 23, 617 (2005).
R. P. Bhatta, B. D. Thoms, M. Alevli, V. Woods, and N.
Dietz, Appl. Phys. Lett. 88, 122112 (2006).
R. P. Bhatta, B. D. Thoms, M. Alevli, and N. Dietz, Surf.
Sci. 601, L120 (2007).
C. Tindall, and J.C. Hemminger, Surf. Sci. 330, 67
S. Tanaka, M. Onchi, and M. Nishijima, Surf.Sci.191,
H. Nienhaus, S. P. Grabowski, and W. Monch, Surf. Sci.
368, 196 (1996).
J. Fritsch, A. Echert, P. Pavone, and U. Schroder, J.
Phys.: Condens. Matter 7, 7717 (1995).